Ternary Rare-Earth Titanium Antimonides RE2Ti11-xSb14+x (RE= Sm, Gd, Tb, Yb)
Haiying Bie; Arthur Mar; Inorganic Chemistry 47 (2008) 6763–6770; doi:10.1021/ic800317c

data_4305325
_publ_contact_author_address
; Department of Chemistry
  University of Alberta
  Edmonton, AB
  Canada  T6G 2G2
;
_publ_contact_author_email       arthur.mar@ualberta.ca
_publ_contact_author_fax         '(780) 492-8231'
_publ_contact_author_name        'Dr. Arthur Mar'
_publ_contact_author_phone       '(780) 492-5592'
_publ_section_title
;
Ternary Rare-Earth Titanium Antimonides RE2Ti11-xSb14+x (RE=
Sm, Gd, Tb, Yb)
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              6763
_journal_page_last               6770
_journal_paper_doi               10.1021/ic800317c
_journal_volume                  47
_journal_year                    2008
_chemical_formula_structural     'Tb2 Ti10.40 Sb14.60'
_chemical_formula_sum            'Sb14.6 Tb2 Ti10.4'
_chemical_formula_weight         2593.55
_chemical_name_common            'terbium titanium antimonide (2/11/14)'
_chemical_name_systematic        'terbium titanium antimonide (2/11/14)'
_space_group_IT_number           62
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   15.8693(18)
_cell_length_b                   5.7036(6)
_cell_length_c                   12.9309(15)
_cell_measurement_reflns_used    3403
_cell_measurement_temperature    295(2)
_cell_measurement_theta_max      32.76
_cell_measurement_theta_min      3.15
_cell_volume                     1170.4(2)
_computing_cell_refinement       'Bruker SAINT 7.06 (Bruker, 2004)'
_computing_data_collection       'Bruker SMART 5.054 (Bruker, 1999)'
_computing_data_reduction        'Bruker SAINT 7.06'
_computing_molecular_graphics    'ATOMS 5.1 (Dowty, 1999)'
_computing_publication_material  'Bruker SHELXTL 6.12'
_computing_structure_refinement  'Bruker SHELXTL 6.12'
_computing_structure_solution    'Bruker SHELXTL 6.12'
_diffrn_ambient_temperature      295(2)
_diffrn_measured_fraction_theta_full 0.991
_diffrn_measured_fraction_theta_max 0.991
_diffrn_measurement_device_type  'Bruker Platform/SMART 1000 CCD'
_diffrn_measurement_method       '\w scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0816
_diffrn_reflns_av_sigmaI/netI    0.0480
_diffrn_reflns_limit_h_max       24
_diffrn_reflns_limit_h_min       -24
_diffrn_reflns_limit_k_max       8
_diffrn_reflns_limit_k_min       -8
_diffrn_reflns_limit_l_max       19
_diffrn_reflns_limit_l_min       -19
_diffrn_reflns_number            15600
_diffrn_reflns_theta_full        33.13
_diffrn_reflns_theta_max         33.13
_diffrn_reflns_theta_min         2.03
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    25.768
_exptl_absorpt_correction_T_max  0.2923
_exptl_absorpt_correction_T_min  0.0758
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   'Bruker SHELXTL 6.12 (Sheldrick, 2001)'
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    7.359
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       prism
_exptl_crystal_F_000             2207
_exptl_crystal_size_max          0.11
_exptl_crystal_size_mid          0.08
_exptl_crystal_size_min          0.05
_refine_diff_density_max         2.186
_refine_diff_density_min         -2.115
_refine_diff_density_rms         0.453
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.052
_refine_ls_matrix_type           full
_refine_ls_number_parameters     92
_refine_ls_number_reflns         2396
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.052
_refine_ls_R_factor_all          0.0554
_refine_ls_R_factor_gt           0.0327
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0223P)^2^+1.0802P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0566
_refine_ls_wR_factor_ref         0.0614
_reflns_number_gt                1866
_reflns_number_total             2396
_reflns_threshold_expression     I>2\s(I)
_cod_data_source_file            ic800317c-file002_3.cif
_cod_data_source_block           Tb2Ti11Sb14
_cod_original_formula_sum        'Sb14.60 Tb2 Ti10.40'
_cod_database_code               4305325